Suppression of Forward Electron Injection from
Ru(dcbpy)2(NCS)2 to Nanocrystalline TiO2 Film
As a Result of an Interfacial Al2O3 Barrier Layer Prepared
with Atomic Layer Deposition
Liisa J. Antila,† Mikko J. Heikkil€,‡ Viivi Aumanen,† Marianna Kemell,‡ Pasi Myllyperkio,†
Markku Leskel€, and Jouko E. I. Korppi-Tommola*
Department of Chemistry, Nanoscience Center, P.O. Box 35, 40014 University of Jyv€skyl€, Finland and
Laboratory of Inorganic Chemistry, Department of Chemistry, P.O. Box 55, 00014 University of Helsinki, Finland
ABSTRACT Subnanometer-thick Al2O3 barrier layers on nanocrystalline TiO2
film were prepared with atomic layer deposition (ALD). The method allowed
variation of barrier thicknesses at atomic resolution also deep in nanoporous
structures, which makes it a superior method as compared to, e.g., sol-gel
techniques. In this letter we present results on the effect of Al2O3 barriers of
various thicknesses on forward electron injection in dye-sensitized solar cells. A
decrease in the amplitude of the oxidized Ru(dcbpy)2(NCS)2 dye absorption signal
due to singlet injection was observed already after one deposition cycle that
produces a discontinuous layer with nominal thickness of 1 Å. More than two
layer coatings also slowed down the triplet injection. The findings indicate
suppression of total electron injection, which is probably due to the Al2O3-induced
weakening of electronic coupling between the dye and TiO2 as well as modification
of the TiO2 electronic structure.
SECTION Kinetics, Spectroscopy
lectron transfer from the excited state of ruthenium have been studied as potential barrier materials, e.g.,
complex dye (Ru(dcbpy)2(NCS)2, also called RuN3, Al2O3,8-12,14 ZrO2,8 SiO2,8 and ZnO.13 While the effect of
dcbpy = 4,40 -dicarboxy-2,20 -bipyridine1) to the con- these materials on recombination rates and power conver-
duction band of the semiconductor (TiO2) is one of the key sion efficiency of the DSSC has been extensively studied, few
processes determining the current output from dye-sensitized reports on their effect on forward electron injection rates
solar cells (DSSCs).2 After excitation the RuN3 singlet state exist.14
undergoes ultrafast electron injection to the semiconductor In liquid-phase methods (the primary methods applied to
(∼50 fs) and intersystem crossing (∼70 fs) to triplet state Al2O3 layer preparation in DSSC, e.g., surface sol-gel
localized on the bipyridine ligands of the RuN3 molecule.3-5 processes15), incomplete penetration of the solution to the
The injection from the triplet state is a heterogeneous process nanoporous TiO2 film results in an uneven coverage of the
occurring on a picosecond time scale.6 The excited state nanosized cavities of the semiconductor.14 Chemical vapor
absorption of the dye attached on TiO2 occurs in the wave- phase methods, such as atomic layer deposition (ALD),16,20
length region of 630-760 nm and that of oxidized dye occurs allow the reactants to penetrate even the most distant nano-
from 760 to 940 nm with correlated time evolution, which is pores near the interface between the semiconductor film and
indicative of a reactant-to-product reaction.4,7 The oxidized the conducting layer of the substrate11 as was found in a
dye absorption dominates over triplet state absorption at Rutherford back-scattering (RBS) measurement of a 8 nm
860 nm as evidenced by an isosbestic point in the excited thick ALD-Al2O3 film on nanoporous TiO2 (data not shown).
state absorption signal of RuN3 dye in solution at this wave- ALD is based on sequential surface reactions where precur-
length. Thus, 860 nm is an ideal probe wavelength for sors react with the surface in a saturative manner. This allows
oxidized dye formation. production of smooth, continuous films and straightforward
Recombination reactions of the injected electron with the control of the thickness of the deposited film by adjusting the
oxidizing agent of the electrolyte (I3-) limit the photocurrent
of the DSSC. As an effort to suppress recombination, the
nanocrystalline semiconductor film has been coated with Received Date: November 23, 2009
high band gap metal oxide layers, which act as barriers for Accepted Date: December 21, 2009
the interfacial electron transfer. Several metal oxide materials Published on Web Date: December 29, 2009
r 2009 American Chemical Society 536 DOI: 10.1021/jz9003075 |J. Phys. Chem. Lett. 2010, 1, 536–539
number of reaction cycles. In the TMA/H2O process20 used in ∼25% is due to the excited state absorption remaining after
this work, the growth per cycle is ∼1 Å. As a result of the singlet injection.4,17 It is obvious from Figure 1 that the signal
saturative nature of ALD, surface reactions allow rather reli- amplitude in the time domain τ >1 ps up to 200 ps also
able calculation of layer thicknesses from growth per cycle diminishes as the barrier thickness increases, leading to a
(see Supporting Information). For submonolayer films, i.e., decrease in the quantum yield of triplet injection as well.3,4
films deposited with less than five deposition cycles, only Vibrational relaxation of related ruthenium complexes has
nominal thicknesses can be estimated since the submono- been reported to take place in a few picoseconds,18 and these
layer films are discontinuous. To our knowledge, ALD has processes may well compete with the slow injection channel.
been applied to barrier layer preparation in DSSCs only in a The quantum yield of the total electron injection can be
few cases.10-12 We report the first study of the effect of ALD determined by calculating the contribution of the oxidized
Al2O3 barrier layers on the forward electron injection from dye to the total signal from the data in Figure 1 according to14
RuN3 dye to the conduction band of TiO2 as a function of
barrier thickness by femtosecond transient absorption spec- Sð860 nm, tÞ ¼ Nex ðtÞAex ð860 nm, tÞ þ Nox ðtÞAox ð860 nmÞ
All samples were sensitized to the same optical density
(absorbance) 0.5 OD. This allows us to compare the ampli- where S(860 nm, t) is the measured signal at time t and at the
tudes of the transient absorption signals directly. In Figure 1, given wavelength and Nex(t) and Nox(t) represent the relative
signals from excited state absorption of the dye and absorp- populations of the excited state and the oxidized form of the
tion of the oxidized dye are shown in two time domains. In dye, respectively. Aex(860 nm, t) is the time-dependent
the region of singlet injection (τ < 1 ps), the signal amplitude absorption of the excited state, i.e., that of the RuN3/Al2O3
decreases as the barrier thickness increases.3,4 The smaller sample, and Aox(860 nm) is the absorption of the oxidized dye
the amplitude (Table 1) the smaller the oxidized dye number determined from the RuN3/TiO2 signal at 520 ps, i.e., after
density in the excitation volume after excitation. This de- injection has completed. For the excited state, a time-depen-
crease in amplitude implies suppression of the fast electron dent absorption signal is used because of the small decay due
injection from the singlet state of the dye. The oxidized to vibrational energy relaxation, while a constant value can be
dye absorption accounts for ∼75% of the amplitude of the used for the oxidized dye because it has no significant time
transient absorption signal in this spectral range, and the dependence. The amplitude of the oxidized dye signal directly
represents the quantum yield of electron injection, and from
Figure 2 it can be seen that the quantum yield decreases by
15% after the first deposition cycle of Al2O3 and falls 70%
with five deposition cycles, i.e., a monolayer of Al2O3.
The electron injection from the dye to the semiconductor
follows the classical Marcus electron transfer theory in the
nonadiabatic limit. The slowing down of injection as electro-
nic coupling between the dye and the semiconductor weak-
ens has been demonstrated by Asbury et al.19 with the
introduction of CH2 spacer groups between the bipyridine
and the semiconductor binding carboxylate groups. The Al2O3
barrier layer also increases the distance between the electron
donating bipyridine orbitals of the dye and the conduction
band of TiO2, leading to weaker electronic coupling. The
gradual decrease of the transient absorption amplitude
(Figure 1) may be due to the discontinuous nature of the
layers prepared with less than five deposition cycles (<5 Å
Figure 1. Time dependencies of the absorbance changes (in nominal thickness).20 It is possible that some dye molecules
mOD) of excited state of the RuN3 dye and of the oxidized dye are still able to bind to TiO2 in samples where the barrier is
probed at 860 nm after 540 nm excitation on uncoated TiO2, on
TiO2 with Al2O3 barrier layers, and on Al2O3. Solid lines are prepared with one or two deposition cycles, and these con-
exponential fits to the experimental data (symbols). sequently have stronger average electronic coupling than
Table 1. Oxidized Dye Formation Time Constants (τ) and Relative Amplitudes (In Percentages of the Total Amplitude) on Bare TiO2 and
Al2O3 Films and Al2O3-Coated TiO2 Films Obtained from Fitting the Data in Figure 1a
TiO2 1 cycle of Al2O3 2 cycles of Al2O3 3 cycles of Al2O3 5 cycles of Al2O3 Al2O3
instrument limited rise 68% 71% 70% 80% 91% 100%
τ1 (ps) 1.2 ( 0.1 (-11%) 1.2 ( 0.1 (-10) 1.2 ( 0.1 (-10%) 3.9 ( 0.4 (-11%) 26 ( 3 (-9%) 25 ( 3 (19%)
τ2 (ps) 11.0 ( 1.1 (-3%) 11.0 ( 1.1 (-8%) 11.0 ( 1.1 (-7%) 145 ( 15 (-9%)
τ3 (ps) 95 ( 10 (-18%) 95 ( 10 (-10%) 95 ( 10 (-13%)
Time resolution of the present experiment did not allow resolving the fast singlet injection rate, which is buried under the instrument limited rise.3,4
Decay amplitudes are given in parentheses.
r 2009 American Chemical Society 537 DOI: 10.1021/jz9003075 |J. Phys. Chem. Lett. 2010, 1, 536–539
In conclusion, we have shown already that one ALD cycle
of Al2O3 results in a barrier that slows down electron injection
from the singlet excited state of RuN3 dye and decreases the
overall injection efficiency. With more than three ALD cycles
of Al2O3, the triplet state injection is also suppressed, indicat-
ing a shift in the TiO2 density of states.
SUPPORTING INFORMATION AVAILABLE TiO2 thin film
preparation, ALD of Al2O3 barrier layers, sensitization with RuN3,
and time-resolved transient absorption spectroscopy (PDF).
This material is available free of charge via the Internet at http://
Figure 2. Injection yields calculated using eq 1 from the data in *To whom correspondence should be addressed. E-mail: jouko.
Figure 1. The numbers are total electron injection yields relative to email@example.com.
samples where the dye binds only to Al2O3. If the dye is ACKNOWLEDGMENT Support from the FinNano research
unable to bind to TiO2 even after one deposition cycle, then program of the Academy of Finland (Contract Nos. 117969 and
the increasing distance with increasing number of deposition 118040) is acknowledged. L.A. is grateful for support from the
cycles would explain the gradual change in electronic cou- Graduate School of Computational Chemistry and Molecular
pling and the observed amplitude. A more detailed study of Spectroscopy and acknowledges Ph.D. Jani Kallioinen for helpful
the slowing down of electron transfer as a function of barrier discussions. Ph.D. Timo Sajavaara is gratefully acknowledged for
layer thickness will be presented elsewhere. RBS measurements.
The injection kinetics on a picosecond time scale of the
samples with one and two cycles of Al2O3 are almost identical
as compared to the kinetics on uncoated TiO2 film, while in
samples with three or more deposition cycles the triplet (1) Nazeeruddin, M. K.; Kay, A.; Rodicio, I.; Humphry-Baker, R.;
injection is suppressed (Table 1). The efficiency of the triplet Mueller, E.; Liska, P.; Vlachopoulos, N.; Graetzel, M. Conver-
state injection is dependent on the conduction band ener- sion of Light to Electricity by cis-X2Bis(2,20 -bipyridyl-4,40 -
getics of the semiconductor. For the N3-TiO2 system, the low- dicarboxylate)ruthenium(II) Charge-Transfer Sensitizers (X =
Cl-, Br-, I-, CN-, and SCN-) on Nanocrystalline Titanium
energy triplet states of the dye lie below the conduction band
Dioxide Electrodes. J. Am. Chem. Soc. 1993, 115, 6382–
edge and are thus associated with slow, possibly thermally 6390.
activated electron transfer. This was found in studies where (2) O0 Regan, B.; Graetzel, M. A Low-Cost, High-Efficiency Solar
slower triplet injection kinetics resulted from excitation of the Cell Based on Dye-Sensitized Colloidal Titanium Dioxide
dye in the red part of its absorption spectrum compared to Films. Nature 1991, 353, 737–740.
excitation at maximum absorption.17 A shift in the conduc- (3) Benko, G.; Kallioinen, J.; Korppi-Tommola, J.; Yartsev, A. P.;
tion band energy of TiO2 will change the density of electron Sundstrom, V. Photoinduced Ultrafast Dye-to-Semiconductor
accepting states with respect to the excite state energy level of Electron Injection from Nonthermalized and Thermalized
the dye and this will appear as a change in injection kinetics - Donor States. J. Am. Chem. Soc. 2002, 124, 489–493.
especially in the picosecond time scale (injection from triplet (4) Kallioinen, J.; Benko, G.; Sundstrom, V.; Korppi-Tommola, J.;
Yartsev, A. P. Electron Transfer from the Singlet and Triplet
state). The band energetics of TiO2 show Nernstian pH- Excited States of Ru(dcbpy)2(NCS)2 into Nanocrystalline TiO2
depedence.21 Being an alkaline coating material (isoelectric Thin Films. J. Phys. Chem. B 2002, 106, 4396–4404.
point 8-9),22 Al2O3 also shifts the TiO2 energy levels up- (5) De Angelis, F.; Fantacci, S.; Selloni, A.; Nazeeruddin, M. K.;
ward.11-13 Lin et al. have studied this effect with ultraviolet Graetzel, M. Time-Dependent Density Functional Theory
photoelectron spectroscopy.11 They suggested that after two Investigations on the Excited States of Ru(II)-Dye-Sensitized
deposition cycles of Al2O3, the dye lowest unoccupied molec- TiO2 Nanoparticles: The Role of Sensitizer Protonation. J. Am.
ular orbital (LUMO) would still remain above the TiO2 Fermi Chem. Soc. 2007, 129, 14156–14157.
level, but after five cycles the Fermi level rises above the (6) Benko, G.; Kallioinen, J.; Myllyperkio, P.; Trif, F.; Korppi-
LUMO, impeding electron injection. Our results are consistent Tommola, J.; Yartsev, A. P.; Sundstrom, V. Interligand Electron
Transfer Determines Triplet Excited State Electron Injection
with this picture in the sense that we observe suppression of
in RuN3-Sensitized TiO2 Films. J. Phys. Chem. B 2004, 108,
the triplet state injection in samples with three or more 2862–2867.
deposition cycles of Al2O3. However, since somewhat efficient (7) Pellnor, M.; Myllyperki€, P.; Korppi-Tommola, J.; Yartsev, A.;
injection is still taking place in the sample with five deposition Sundstr€m, V. Photoinduced Interfacial Electron Injection in
cycles of Al2O3, we doubt that the Fermi level would have RuN3-TiO2 Thin Films: Resolving Picosecond Timescale
risen high enough to be able to halt electron injection as Injection from the Triplet State of the Protonated and Depro-
suggested by Lin et al. tonated Dyes. Chem. Phys. Lett. 2008, 462, 205–208.
r 2009 American Chemical Society 538 DOI: 10.1021/jz9003075 |J. Phys. Chem. Lett. 2010, 1, 536–539
(8) Palomares, E.; Clifford, J. N.; Haque, S. A.; Lutz, T.; Durrant,
J. R. Control of Charge Recombination Dynamics in Dye
Sensitized Solar Cells by the Use of Conformally Deposited
Metal Oxide Blocking Layers. J. Am. Chem. Soc. 2003, 125,
(9) O0 Regan, B. C.; Scully, S.; Mayer, A. C.; Palomares, E.; Durrant,
J. The Effect of Al2O3 barrier Layers in TiO2/Dye/CuSCN
Photovoltaic Cells Explored by Recombination and DOS
Characterization Using Transient Photovoltage Measure-
ments. J. Phys. Chem. B 2005, 109, 4616–4623.
(10) Law, M.; Greene, L. E.; Radenovic, A.; Kuykendall, T.;
Liphardt, J.; Yang, P. ZnO-Al2O3 and ZnO-TiO2 Core-Shell
Nanowire Dye-Sensitized Solar Cells. J. Phys. Chem. B 2006,
(11) Lin, C.; Tsai, F.; Lee, M.; Lee, C.; Tien, T.; Wang, L.; Tsai, S.
Enhanced Performance of Dye-Sensitized Solar Cells by
an Al2O3 Charge-Recombination Barrier Formed by Low-
Temperature Atomic Layer Deposition. J. Mater. Chem.
2009, 19, 2999–3003.
(12) Tien, T.; Pan, F.; Wang, L.; Lee, C.; Tung, Y.; Tsai, S.; Lin, C.;
Tsai, F.; Chen, S. Interfacial Energy Levels and Related Proper-
ties of Atomic-Layer-Deposited Al2O3 Films on Nanoporous
TiO2 Electrodes of Dye-Sensitized Solar Cells. Nanotechnology
2009, 20, 305201/1–305201/8.
(13) Diamant, Y.; Chappel, S.; Chen, S. G.; Melamed, O.; Zaban, A.
Core-Shell Nanoporous Electrode for Dye Sensitized Solar Cells:
The Effect of Shell Characteristics on the Electronic Properties of
the Electrode. Coord. Chem. Rev. 2004, 248, 1271–1276.
(14) Guo, J.; She, C.; Lian, T. Effect of Insulating Oxide Overlayers
on Electron Injection Dynamics in Dye-Sensitized Nanocrys-
talline Thin Films. J. Phys. Chem. C 2007, 111, 8979–8987.
(15) Ichinose, I.; Senzu, H.; Kunitake, T. A Surface Sol-Gel Process
of TiO2 and Other Metal Oxide Films with Molecular Preci-
sion. Chem. Mater. 1997, 9, 1296–1298.
(16) Ritala, M.; Niinist€, J. Atomic Layer Deposition. In Chemical
Vapour Deposition: Precursors, Processes and Applications;
Jones, A. C., Hitchman, M. L., Eds.; The Royal Society of
Chemistry: Cambridge, U.K., 2009; Chapter 4, pp 128-206.
(17) Myllyperkioe, P.; Benko, G.; Korppi-Tommola, J.; Yartsev, A.
P.; Sundstroem, V. A Study of Electron Transfer in Ru(dcbpy)2-
(NCS)2 Sensitized Nanocrystalline TiO2 and SnO2 Films
Induced by Red-Wing Excitation. Phys. Chem. Chem. Phys.
2008, 10, 996–1002.
(18) Lehtovuori, V.; Aumanen, J.; Myllyperkioe, P.; Rini, M.;
Nibbering, E. T. J.; Korppi-Tommola, J. Transient Midinfrared
Study of Light Induced Dissociation Reaction of Ru(dcbpy)-
(CO)2I2 in Solution. J. Phys. Chem. A 2004, 108, 1644–1649.
(19) Asbury, J. B.; Hao, E.; Wang, Y.; Ghosh, H. N.; Lian, T.
Parameters Affecting Electron Injection Dynamics from
Ruthenium Dyes to Titanium Dioxide Nanocrystalline Thin
Film. J. Phys. Chem. B 2001, 105, 4545–4557.
(20) Puurunen, R. L. Surface Chemistry of Atomic Layer Deposi-
tion: A Case Study for the Trimethylaluminum/Water Process.
J. Appl. Phys. 2005, 97, 121301/1–121301/52.
(21) Rothenberger, G.; Fitzmaurice, D.; Graetzel, M. Spectroscopy
of Conduction Band Electrons in Transparent Metal Oxide
Semiconductor Films: Optical Determination of the Flatband
Potential of Colloidal Titanium Dioxide Films. J. Phys. Chem.
1992, 96, 5983–5986.
(22) Kosmulski, M. Attempt To Determine Pristine Points of Zero
Charge of Nb2O5, Ta2O5, and HfO2. Langmuir 1997, 13,
r 2009 American Chemical Society 539 DOI: 10.1021/jz9003075 |J. Phys. Chem. Lett. 2010, 1, 536–539